Bismuth telluride

Single crystal of bismuth telluride

Atomic structure: ideal (l) and with a twin defect (r)

Electron micrograph of twinned bismuth telluride

Identifiers

CAS Number

* 1304-82-1 Y

3D model (JSmol)

* Interactive image

ChemSpider |

* 11278988 Y

ECHA InfoCard | 100.013.760
EC Number |

* 215-135-2

PubChem CID

* 6379155

UNII |

* 1818R19OHO Y

CompTox Dashboard (EPA)

* DTXSID90894839

InChI

* InChI=1S/2Bi.3Te/q2*+3;3*-2 Y

Key: AZFMNKUWQAGOBM-UHFFFAOYSA-N Y

* InChI=1/2Bi.3Te/q2*+3;3*-2

Key: AZFMNKUWQAGOBM-UHFFFAOYAF

SMILES

* [Te-2].[Te-2].[Te-2].[Bi+3].[Bi+3]

Properties

Chemical formula

| Bi2Te3
Molar mass | 800.76 g·mol−1
Appearance  | Grey powder or metallic grey crystals
Density | 7.74 g/cm3[1]
Melting point | 580 °C (1,076 °F; 853 K)[1]

Solubility in water

| insoluble[1]
Solubility in ethanol | soluble[1]
Structure

Crystal structure

| Trigonal, hR15

Space group

| R3m, No. 166[2]

Lattice constant

a = 0.4395 nm, c = 3.044 nm

Formula units (Z)

| 3
Hazards
NFPA 704 (fire diamond)  |

Flash point | noncombustible[3]
NIOSH (US health exposure limits):

PEL (Permissible)

| TWA 15 mg/m3 (total) TWA 5 mg/m3 (resp) (pure)
none (doped with selenium sulfide) [3]

REL (Recommended)

| TWA 10 mg/m3 (total) TWA 5 mg/m3 (resp) (pure) TWA 5 mg/m3 (doped with selenium sulfide)[3]

IDLH (Immediate danger)

| N.D. (pure and doped)[3]
Safety data sheet (SDS)  | Sigma-Aldrich
Related compounds

Other anions

* Bismuth(III) oxide
* Bismuth trisulfide
* Bismuth selenide

Other cations

| Arsenic telluride
Antimony telluride

Except where otherwise noted, data are given for materials in their standard state (at 25 °C [77 °F], 100 kPa).

N verify (what is YN ?)

Infobox references

Chemical compound

Bismuth telluride (Bi2Te3) is a gray powder that is a compound of bismuth and tellurium also known as bismuth(III) telluride. It is a semiconductor, which, when alloyed with antimony or selenium, is an efficient thermoelectric material for refrigeration or portable power generation. Bi2Te3 is a topological insulator, and thus exhibits thickness-dependent physical properties.

## Properties as a thermoelectric material[edit]

Bismuth telluride is a narrow-gap layered semiconductor with a trigonal unit cell. The valence and conduction band structure can be described as a many-ellipsoidal model with 6 constant-energy ellipsoids that are centered on the reflection planes.[4] Bi2Te3 cleaves easily along the trigonal axis due to Van der Waals bonding between neighboring tellurium atoms. Due to this, bismuth-telluride-based materials used for power generation or cooling applications must be polycrystalline. Furthermore, the Seebeck coefficient of bulk Bi2Te3 becomes compensated around room temperature, forcing the materials used in power-generation devices to be an alloy of bismuth, antimony, tellurium, and selenium.[5]

Recently, researchers have attempted to improve the efficiency of Bi2Te3-based materials by creating structures where one or more dimensions are reduced, such as nanowires or thin films. In one such instance n-type bismuth telluride was shown to have an improved Seebeck coefficient (voltage per unit temperature difference) of −287 μV/K at 54 °C,[6] However, one must realize that Seebeck coefficient and electrical conductivity have a tradeoff: a higher Seebeck coefficient results in decreased carrier concentration and decreased electrical conductivity.[7]

In another case, researchers report that bismuth telluride has high electrical conductivity of 1.1×105 S·m/m2 with its very low lattice thermal conductivity of 1.20 W/(m·K), similar to ordinary glass.[8]

## Properties as a topological insulator[edit]

Bismuth telluride is a well-studied topological insulator. Its physical properties have been shown to change at highly reduced thicknesses, when its conducting surface states are exposed and isolated. These thin samples are obtained through either epitaxy or mechanical exfoliation.

Epitaxial growth methods such as molecular beam epitaxy and metal organic chemical vapor deposition are common methods of obtaining thin Bi2Te3 samples. The stoichiometry of samples obtained through such techniques can vary greatly between experiments, so Raman spectroscopy is often used to determine relative purity. However, thin Bi2Te3 samples are resistant to Raman spectroscopy due to their low melting point and poor heat dispersion.[9]

The crystalline structure of Bi2Te3 allows for mechanical exfoliation of thin samples by cleaving along the trigonal axis. This process is significantly lower in yield than epitaxial growth, but produces samples without defects or impurities. Similar to extracting graphene from bulk graphite samples, this is done by applying and removing adhesive tape from successively thinner samples. This procedure has been used to obtain Bi2Te3 flakes with a thickness of 1 nm.[10] However, this process can leave significant amounts of adhesive residue on a standard Si/SiO2 substrate, which in turn obscure atomic force microscopy measurements and inhibit the placement of contacts on the substrate for purposes of testing. Common cleaning techniques such as oxygen plasma, boiling acetone and isopropyl alcohol are ineffective in removing residue.[11]

## Occurrence and preparation[edit]

This section does not cite any sources. Please help improve this section by adding citations to reliable sources. Unsourced material may be challenged and removed.
Find sources: "Bismuth telluride" – news · newspapers · books · scholar · JSTOR (December 2019) (Learn how and when to remove this template message)

|

The mineral form of Bi2Te3 is tellurobismuthite which is moderately rare. There are many natural bismuth tellurides of different stoichiometry, as well as compounds of the Bi-Te-S-(Se) system, like Bi2Te2S (tetradymite).

Bismuth telluride may be prepared simply by sealing mixed powders of bismuth and tellurium metal in a quartz tube under vacuum (critical, as an unsealed or leaking sample may explode in a furnace) and heating it to 800 °C in a muffle furnace.

## See also[edit]

* Thermoelectric materials
* Thermoelectric effect
* Topological insulator

## References[edit]

1. ^ a b c d Haynes, William M., ed. (2011). CRC Handbook of Chemistry and Physics (92nd ed.). Boca Raton, FL: CRC Press. p. 4.52. ISBN 1-4398-5511-0.
2. ^ Feutelais, Y.; Legendre, B.; Rodier, N.; Agafonov, V. (1993). "A study of the phases in the bismuth – tellurium system". Materials Research Bulletin. 28 (6): 591. doi:10.1016/0025-5408(93)90055-I.
3. ^ a b c d NIOSH Pocket Guide to Chemical Hazards. "#0056". National Institute for Occupational Safety and Health (NIOSH).
4. ^ Caywood, L. P.; Miller, G. (1970). "Anisotropy of the constant energy surfaces in p-type Bi2Te3 and Bi2Se3 from galvanomagnetic coefficients". Phys. Rev. B. 2 (8): 3209. Bibcode:1970PhRvB...2.3209C. doi:10.1103/PhysRevB.2.3209.
5. ^ Satterthwaite, C. B.; Ure, R. (1957). "Electrical and Thermal Properties of Bi2Te3". Phys. Rev. 108 (5): 1164. Bibcode:1957PhRv..108.1164S. doi:10.1103/PhysRev.108.1164.
6. ^ Tan, J. (2005). "Thermoelectric properties of bismuth telluride thin films deposited by radio frequency magnetron sputtering". Proceedings of SPIE. Proceedings of the SPIE. Smart Sensors, Actuators, and MEMS II. Vol. 5836\. pp. 711–718. Bibcode:2005SPIE.5836..711T. doi:10.1117/12.609819. S2CID 123199126.
7. ^ Goldsmid, H. J.; Sheard, A. R. & Wright, D. A. (1958). "The performance of bismuth telluride thermojunctions". Br. J. Appl. Phys. 9 (9): 365. Bibcode:1958BJAP....9..365G. doi:10.1088/0508-3443/9/9/306.
8. ^ Takeiishi, M.; et al. "Thermal conductivity measurements of Bismuth Telluride thin films by using the 3 Omega method" (PDF). The 27th Japan Symposium on Thermophysical Properties, 2006, Kyoto. Archived from the original (PDF) on 2007-06-28. Retrieved 2009-06-06.
9. ^ Teweldebrhan, D.; Goyal, V.; Balandin, A. A (2010). "From Graphene to Bismuth Telluride: Mechanical Exfoliation of Quasi-2D Crystals for Applications in Thermoelectrics and Topological Insulators". Nano Letters. 10 (12): 1209–18. Bibcode:2010NanoL..10.1209T. doi:10.1021/nl903590b. PMID 20205455.
10. ^ Teweldebrhan, Desalegne; Balandin, Alexander A. (2010). ""Graphene-Like" Exfoliation of Atomically-Thin Films of Bi". ECS Transactions: 103–117. doi:10.1149/1.3485611. S2CID 139017503.
11. ^ Childres, Isaac; Tian, Jifa; Miotkowski, Ireneusz; Chen, Yong (2013). "AFM and Raman studies of topological insulator materials subject to argon plasma etching". Philosophical Magazine. 93 (6): 681–689. arXiv:1209.2919. Bibcode:2013PMag...93..681C. doi:10.1080/14786435.2012.728009. S2CID 38149843.

## External links[edit]

* Media related to Bismuth telluride at Wikimedia Commons
* Bismuth Telluride and its Alloys (Chapter 4.5 of Martin Wagner dissertation)
* CDC – NIOSH Pocket Guide to Chemical Hazards – Bismuth Telluride, undoped

* v
* t
* e

Bismuth compounds

Bismuth(III)|

* BiBr3
* BiCl3
* Bi4Ge3O12
* BiOCl
* BiOI
* BiONO3
* Bi2Se3
* Bi12SiO20
* Bi2O2(CO3)
* Bi2Te3
* BiF3
* BiI3
* Bi(NO3)3
* Bi2O3
* BiP
* Bi(OH)3
* Bi2S3
* BiH3
* subsalicylate
* subcitrate

| Organobismuth(III)|

* C4H4BiH

|

Bismuth(V)|

* NaBiO3
* BiF5
* Bi2O5

* v
* t
* e

Tellurides

| H2Te |  |  |  |  |  |  |  |  |  |  |  |  |  |  |  |  |  | He

|
|
|
|
|
|
|
|
|
|
|
|
|
|
|
|
|
|

Li2Te | BeTe |  |  |  |  |  |  |  |  |  |  |  | B  | CTe2
(CH3)2Te | (NH4)2Te | O  | F  | Ne
Na2Te | MgTe |  |  |  |  |  |  |  |  |  |  |  | Al2Te | Si  | P0.8Te0.2 | S  | Cl  | Ar
K2Te | CaTe |  | Sc2Te3 | Ti  | VTe2 | CrTe
Cr2Te3 | MnTe
MnTe2 | FeTe | CoTe | NiTe | Cu2Te
CuTe
CuTe2 | ZnTe | GaTe
Ga2Te3
-Ga | GeTe
-Ge | As2Te3
As4Te3 | Se  | +Br | Kr
Rb2Te | SrTe |  | Y2Te3 | ZrTe5 | NbTe2 | MoTe2 | Tc  | Ru  | Rh  | Pd  | Ag2Te | CdTe | In2Te3 | SnTe
SnTe2 | Sb2Te3 | Te2-
Te2-
n | I  | Xe
Cs2Te | BaTe | *  | Lu  | HfTe5 | TaTe2 | WTe2
WTe3 | ReTe2 | Os  | Ir  | Pt  | AuxTey | HgTe | Tl2Te | PbTe | Bi2Te3 | Po  | At  | Rn
Fr  | RaTe | **  | Lr  | Rf  | Db  | Sg  | Bh  | Hs  | Mt  | Ds  | Rg  | Cn  | Nh  | Fl  | Mc  | Lv  | Ts  | Og  |  |  |  |  |  |  |  |
|  | ↓ |  |  |  |  |  |  |  |  |  |  |  |  |  |  |
|  | * | La2Te3 | Ce2Te3 | Pr2Te3 | Nd2Te3 | Pm  | Sm2Te3 | EuTe
Eu2Te3 | Gd  | Tb  | Dy  | Ho  | Er2Te3 | Tm2Te3 | Yb  |
|  | ** | Ac  | ThTe2 | Pa  | UTe2 | Np  | Pu  | Am  | Cm  | Bk  | Cf  | Es  | Fm  | Md  | No  |
*[CID]: Compound ID
*[EPA]: U.S. Environmental Protection Agency
*[v]: View this template
*[t]: Discuss this template
*[e]: Edit this template